Common Name(s): Alder-leaf Birch
Scientific Name: Betula alnoides
Distribution: Burma, India, and Nepal
Tree Size: 65-100 ft (20-30 m) tall, 2-3 ft (.6-1.0 m) trunk diameter
Average Dried Weight: 33 lbs/ft3 (530 kg/m3)
Specific Gravity (Basic, 12% MC): .41, .53
Janka Hardness: 830 lbf (3,690 N)
Modulus of Rupture: 8,980 lbf/in2 (61.9 MPa)
Elastic Modulus: 1,235,000 lbf/in2 (8.52 GPa)
Crushing Strength: 6,400 lbf/in2 (44.1 MPa)
Shrinkage: Radial: 5.0%, Tangential: 7.0%, Volumetric: 13.0%, T/R Ratio: 1.4
Color/Appearance: Heartwood tends to be a light reddish brown, with nearly white sapwood. Occasionally figured pieces are available with a wide, shallow curl similar to the curl found in Cherry. There is virtually no color distinction between annual growth rings, giving Birch a somewhat dull, uniform appearance.
Grain/Texture: Grain is generally straight or slightly wavy, with a fine, even texture. Low natural luster.
Endgrain: Diffuse-porous; primarily radial multiples; medium pores in no specific arrangement, moderately numerous to numerous; parenchyma marginal, and sometimes diffuse-in-aggregates (faintly visible with lens); narrow rays, spacing fairly close to close.
Rot Resistance: Birch is perishable, and will readily rot and decay if exposed to the elements. The wood is also susceptible to insect attack.
Workability: Generally easy to work with hand and machine tools, though boards with wild grain can cause grain tearout during machining operations. Turns, glues, and finishes well.
Odor: No characteristic odor.
Allergies/Toxicity: Birch in the Betula genus has been reported as a sensitizer. Usually most common reactions simply include skin and respiratory irritation. See the articles Wood Allergies and Toxicity and Wood Dust Safety for more information.
Pricing/Availability: Likely to be rather economical in most instances. Figured boards can be more expensive, but normally plain birch lumber is in the same price range as maple or oak.
Sustainability: This wood species is not listed in the CITES Appendices or on the IUCN Red List of Threatened Species.
Common Uses: Plywood, boxes, crates, turned objects, interior trim, and other small specialty wood items.
Comments: Birch is one of the most widely used woods for veneer and plywood worldwide. Besides regular sheets of plywood, Birch veneer is also used for doors, furniture, and paneling.
- Alaska Paper Birch (Betula neoalaskana)
- Downy Birch (Betula pubescens)
- Gray Birch (Betula populifolia)
- Paper Birch (Betula papyrifera)
- River Birch (Betula nigra)
- Silver Birch (Betula pendula)
- Sweet Birch (Betula lenta)
- Yellow Birch (Betula alleghaniensis)
Scans/Pictures: There are currently no pictures of this exact wood species, but a similar species within the Betula genus is being substituted (B. alleghaniensis). If you’d like to contribute a wood sample of this specific species to be scanned, (even small pieces of veneer can be sent), please use the contact form.